systematic electrical characterization study of a hybrid...
Embed Size (px)
ENSENANZA REVISTA MEXICANA DE FISICA E 57 (1) 73–77 JUNIO 2011
Systematic electrical characterization study of a hybrid organic-inorganicsemiconductor heterojunction at different illumination conditions
Oscar H. Salinasa,b, M.C. Arenasc, M.E. Nichod, and Hailin HubaUniversidad Tecnologica Emiliano Zapata del Estado de Morelos,
Av. Universidad Tecnologica No. 1, Col. Palo Escrito, C.P. 62760, Emiliano Zapata, Morelos,e-mail: [email protected]
b Centro de Investigacion en Energıa, Universidad Nacional Autonoma de Mexico,Apartado Postal 34, Temixco 62580, Morelos, Mexico.
cCentro de Fısica Aplicada y Tecnologıa Avanzada, Universidad Nacional Autonoma de Mexico,Apartado Postal 1-1010, Santiago de Queretaro, Queretaro, 76000, Mexico,
e-mail: [email protected] de Investigacion en Ingenierıa y Ciencias Aplicadas, Universidad Autonoma del Estado de Morelos,
Av. Universidad 1001, Col. Chamilpa, 62209, Cuernavaca, Morelos, Mexico.
Recibido el 15 de diciembre de 2010; aceptado el 3 de marzo de 2011
Electrical characterization study of hybrid heterojunctions (HHJs) based on CdS and poly(3octylthiophene) (P3OT) is performed in orderto know the process repeatability and materials homogeneity that may influence on power conversion efficiency (PCE) of CdS/P3OT pho-tovoltaic (PV) solar cells. Basic statistical and numerical techniques for solving linear equations were used for systematic analysis of PVperformance of those HJs. Adjustment curves were calculated from experimental data with the adjustment factor equal to almost 99.9 %,which means that the model has a high confidence level. They also were combined with theoretical models to establish a mathematicalmodel that can describe the electrical performance of the mentioned junctions. PV response was analyzed under different illumination con-ditions, 23, 40, 124 and 285 mW/cm2 of Irr level. The relationships between short circuit current (JSC ) and open circuit voltage (VOC )with irradiance level (Irr) were determined with high confidence level too. The dependence ofJSC on Irr is linear, whereasVOC dependslogarithmically onIrr and onJSC . For spectral response a 100 Watts halogen lamp and light filters from 400 nm to 689 nm of wavelengthwere used. The maximum incident photon converted to electron efficiency (IPCE) was experimentally determined at 2.75 eV of photonenergy. This value corresponds to the optical forbidden gap of the inorganic semiconductor material. The obtained results are in agreementwith the theoretical concepts of PV devices.
Keywords: Photovoltaic effect; short circuit current; open circuit voltage; irradiance.
En este trabajo se realiza un estudio sistematico de la caracterizacion electrica de heterouniones hıbridas con la finalidad de conocer larepetitividad del proceso y la homogeneidad de materiales que se utilizan para preparar dispositivos electronicos semiconductores paraaplicacion fotovoltaica. La caracterizacion electrica de dispositivos fotovoltaicos se realiza para saber su eficiencia de conversion de energıa.Para el analisis sistematico de los resultados electricos, se utilizaron tecnicas basicas estadısticas y de metodos numericos para resolverecuaciones lineales que involucran parametros electricos del dispositivo. Las curvas de ajuste obtenidas a partir de los datos experimentalespresentaron un factor de ajuste del 99.9 %, lo que significa un alto nivel de confianza en el modelo. Estas curvas de ajuste fueron combinadascon modelos teoricos para obtener un modelo matematico que describe el comportamiento electrico de este tipo de uniones especıficas. Larelacion entre la corriente de corto circuito (JSC ) y el voltaje de corto circuito (VOC ) con el nivel de irradiancia (Irr) se determinaron conun alto nivel de confianza. Las curvas demuestran queJSC depende linealmente conIrr, mientras que elVOC depende logarıtmicamente.Por otro lado,VOC depende logarıtmicamente deJSC . La respuesta fovoltaica fue analizada a 23, 40, 124 y 285 mW/cm2 de nivel deirradiancia. Se utilizaron filtros de 400 a 689 nm de longitud de onda y una lampara de halogeno de 100 Watts para obtener la respuestaespectral. La maxima eficiencia de conversion de fotones incidentes (IPCE) se determino experimentalmente en 2.75 eV de energıa de losfotones, valor que corresponde con el ancho de banda prohibida del material semiconductor inorganico. Los resultados obtenidos concuerdancon los conceptos teoricos basicos de dispositivos fotovoltaicos.
Descriptores: Efecto fotovoltaico; corriente a corto circuito; voltaje a circuito abierto; irradiancia.
PACS: 73.50.h; 73.40.c; 73.61.r; 85.60.Bt; 85.60.Dw
Electrical characterization of a semiconductor electronic de-vice is an effective way to get knowledge about the physicalbehavior of each component layer as well as that of the wholejunction. Test conditions depend on the device application,and in the case of PV semiconductor devices electrical char-acterization under dark and illumination conditions are re-
quired. The common procedure is to get the current versusvoltage curves, called I-V curves, for both test conditions.Parameters gotten directly from the I-V curves, are open cir-cuit voltage (VOC) and short circuit current (JSC). The firstone has been related mainly with energy differences levelsat the interface of the electron-acceptor and electron-donormaterials according to a flat energy band analysis . Onthe other hand, theJSC value depends on the generation and
74 O.H. SALINAS, M.C. ARENAS, M.E. NICHO, AND HAILIN HU
FIGURE 1. I-V curves of CdS/P3OT hybrid HJ in dark (solid line)and under illumination conditions (circles) at 88 mW/cm2 of Irr
FIGURE 2. Distributions ofJSC data at differentIrr levels.
collection of the two free charge carriers, electrons and holes.Charge carrier generation could be done by different sources,for instance light and heat. When light is the source thereare two principal parameters that impact on this free chargecarriers generation, light intensity and light wavelength. Thefirst is related to theIrr and can be analyzed from the powerconversion efficiency (PCE) results. The second one is ana-lyzed by calculating the incident photon converted to electronefficiency (IPCE), which is also called internal quantum effi-ciency . Since the amount of available photons varies withthe photon wavelength , reaching to maximum values atvisible region, the IPCE depends on the absorption coeffi-cient and band-gap of absorbing material in a solar cell. Col-lection of free charge carriers depends on the materials prop-erties like mobility, lifetime carrier recombination issues, re-sistivity, and so on . Another two parameters, PCE andfill factor (FF ) are calculated based onVOC andJSC lev-els . PCE is the ratio between the output power and theincident power of the PV devices. Output power, also calledmaximum power, is straightly related to the electrical per-formance of the photovoltaic devices; it is calculated as theproduct ofJSC and VOC . It is also related with theFF ,which depends on the I-V curve shape. Incident power is the
Irr level applied on the front or back surface of PV devices.Based on extracted and calculated PV parameters, the deviceperformance can be evaluated for its PV application. Physicalphenomena occurred in PV devices are so-called photovoltaiceffects, and the conversion from solar energy into electricalenergy is well described in literature [1-5]. Statistical anal-ysis is useful to know process repeatability, semiconductorthin layer homogeneity, and device reliability about its elec-trical performance. Following this kind of analysis, mathe-matical models describing the experimental behavior can begotten based on experimental data and simple correlation andregression analysis.
Organic or polymer PV devices can be prepared usingdifferent types of device structures [6-8]. Heterojunctions(HJs) are one of them. They can be prepared either pla-nar [1,9] (separated electron donor and acceptor layers), orbulk structure (mixed electron donor and acceptor materialsto form a single PV active layer) . There are technolog-ical differences between them, but the main one is the in-terfacial area . About PV cell preparation process, pla-nar heterojunction (HJ) is easier to prepare and to analyzethan bulk HJ. In the organic materials family a bulk HJhas been shown higher PCE than the planar one. In previ-ous works [9,11], we have developed planar HJs based onpoly(3octylthiophene)-cadmium sulfide for photovoltaic ap-plication. A statistical study about the photovoltaic perfor-mance of organic/inorganic HJ is presented in this work.
Hybrid HJs based on planar structures ITO/CdS/P3OT/Cu,were prepared for this statistical study. Transparent conduc-tive ITO substrates were cleaned before CdS layer depositionfollowing the procedure described in Ref. 6. Layers of CdSwere deposited by chemical bath deposition (CBD) [12,13].The obtained CdS layers had a thickness of 200 nm and theywere used as-prepared without any further heat or chemicaltreatment. P3OT in toluene solution was drop-cast on CdSfilm, as described in previous reports [1,14]. The thicknessof deposited P3OT films were about 200 nm, measured onan Atomic Force Microscope (AFM, NanoScope MultimodeScanning Microscope) . P3OT and CdS optical band gap(Eg) is about 1.8 eV and 2.4 eV, respectively [1,12]. TheHighest Occupied Molecular Orbital (HOMO) level and theelectron affinity (χ) of P3OT are 5.4 eV and 3.4 eV, respec-tively .
The top contact of HJs was Cu [1,15]. Cadmium sul-fide (CdS) is the electron acceptor and poly(3octylthiopene)(P3OT) is electron donor in this HJ. The electrical contactbetween CdS and ITO was ohmic behavior . Electri-cal characterization of CdS/P3OT hybrid HJs at 25C in airwas done with an automatic data acquisition system whichconsists in a Keithley 230 programmable voltage source anda Keithley 619 electrometer/multimeter, both coupled eachother and connected to a personal computer. Illuminationof HJ devices was through ITO layer by using a 100 Watts
Rev. Mex. Fıs. E57 (1) (2011) 73–77
SYSTEMATIC ELECTRICAL CHARACTERIZATION STUDY OF A HYBRID ORGANIC-INORGANIC SEMICONDUCTOR. . . 75
TABLE I. Estimated electrical parameter values of different hybrid HJs.
Irr VOC JSC 10−6 J0 10−6 FF Rshunt108 n φB
(mW/cm2) (mV) (mA/cm2) (mA/cm2) (Ω) (eV)
285 211 44.00 0.0884 0.34 8.2 1.53 1.02
124 200 16.40 0.0884 0.422 27 0.71 1.02
40 156 3.40 0.0884 0.398 130 0.79 1.02
23 134 2.63 0.0884 0.327 85 0.83 1.02
285 183 60.6 0.115 0.381 6.0 0.54 1.01
124 164 26.6 0.115 0.338 12 0.57 1.01
40 148 7.74 0.115 0.39 50 0.65 1.01
23 152 4.01 0.115 0.412 140 0.77 1.01
285 117 50.40 0.177 0.291 2.8 0.43 1.00
124 233 16.40 0.177 0.357 28 1.00 1.00
40 196 5.30 0.177 0.388 100 1.10 1.00
23 164 2.84 0.177 0.378 200 1.08 1.00
FIGURE 3. JSC vs. Irr, linear (a) and logarithmic scale (b).
halogen lamp. TheIrr level was 88 mW/cm2, close to84 mW/cm2 corresponding to AM1.5 spectrum . The mea-surement was done at three different zones of each sample inorder to get information about the sample homogeneity. Sta-tistical analysis was performed using free software. Correla-tion and regression analysis was done to get mathematical
FIGURE 4. VOC dependence on theIrr level.
models based on experimental data. These models describeelectrical behavior of hybrids HJs with a high confidencelevel.
The current through PV devices increases significantly whenthe cell samples are under illumination conditions, as showedin Fig. 1. When HJ is in dark there is no electric energy gen-eration (solid line). The I-V curve shows soft trace underillumination conditions, the kind of the trace impacts on theFill Factor (FF ) of the PV devices . Higher values ofFFare expected for soft traces, while resistive traces have lowerFF values. Experimental I-V curve can be modeled usingthe following mathematical model :
Rev. Mex. Fıs. E57 (1) (2011) 73–77
76 O.H. SALINAS, M.C. ARENAS, M.E. NICHO, AND HAILIN HU
FIGURE 5. Logarithmic correlation betweenVOC andJSC .
FIGURE 6. IPCE of the hybrid HJ at different photon wavelengthvalues.
I = IL −[Io
This model is obtained from a basic electrical circuit in-cluding an ideal diode, a series resistance (RS) and a parallelresistance (Rshunt) . As shown in the inset of Fig. 1 thetheoretical and experimental curves match very well. There-fore values of important parameters of HJs can be extractedand estimated, that are listed in Table I. The procedure to getthe barrier height (φB) is explained in literature [1,4]. In thiscase, its value is estimated at 1.0 eV approximately. Accord-ing to the energy flat band diagram, the energy differencebetween Lowest Unoccupied Molecular Orbital (LUMO) ofP3OT and Conduction Band (EC) of CdS is 1 eV approxi-mately . It means that thermionic emission mechanism isdominating in the current transport. It shows in Table I thatthe higher theIrr the higher the influence of theRshunt. Theideality factor (n) has not a clear correlation with theIrr,and in the best of the cases it is 1, which is the ideal case.The reverse saturation current density (J0) does not depend
on theIrr level but on the zone of the sample, which is ex-pected. According to the results showed in Table I, there is adependence of theJSC andVOC values on theIrr. TheJSC
dependence on theIrr level is shown in Fig. 2. It is clearthat the highestJSC is obtained at higherIrr levels. Alsoat higherIrr levels, theJSC data distribution is more open.According to the experimental data, the relationship betweentheJSC andIrr is linear (Fig. 3). The different symbols (tri-angles, squares and circles) correspond to the measurementstaken from three different zones of the samples. Solid linecorresponds to the line of better adjustment of the experimen-tal data. The adjustment factor (R) has a value close to one(0.998 average, inset of Fig. 3a), which means a very goodagreement between the linear adjustment with experimentaldata. Based on that, the relationship betweenJSC andIrr
can be written as follows:
JSC = (0.182Irr − 2.3)10−6 (2)
It can be seen in Fig. 3b that the dependence ofJSC onIrr follows the power law,JSC vs. Iα
rr. Values ofα close toone are expected for PV devices where bimolecular recombi-nation has no impact and therefore transport of hole and elec-tron can be done with comparable efficiency . In this caseα is 1.11, in average, therefore we can declare that bimolec-ular recombination is present. It is also reported that for highIrr levels theJSC magnitude is limited by this mechanism ortends to be saturated.
If the Eq. (1) is analyzed at zero current conditions (opencircuit) and noRS influence, the following equation is ob-tained,
Combining Eq. (2) and Eq. (3),
((0.182Irr − 2.3)10−6
Therefore a logarithmic dependence betweenVOC andIrr level is expected, which can be corroborated in Fig. 4.The use of Eq. (4) to calculate expected values ofVOC basedon Irr measurements could introduce calculate errors, be-cause it does not take into account resistive effects. In or-der to get more accurate estimated values ofVOC based onexperimental data the following equation is used,
IL = IO
Solving Eq. (5), by numerical methods, it is possible toestimateVOC . A comparison between experimental data(different symbols) and estimatedVOC values is shown inFig. 4. The maximum mismatch values is around 3 mV,which means the experimental-theoretical model is very ac-curate.
Rev. Mex. Fıs. E57 (1) (2011) 73–77
SYSTEMATIC ELECTRICAL CHARACTERIZATION STUDY OF A HYBRID ORGANIC-INORGANIC SEMICONDUCTOR. . . 77
On the other hand, the Eq. (4) also indicates a logarith-mic correlation betweenVOC andJSC , which can be corrob-orated in Fig. 5. The analysis of the electrical response withlight of different wavelength is done by calculating the IPCEas follows,
whereλ andIrrλ are the light wavelength and the irradiancelevel at that wavelength, respectively. Units ofJSC could beA (or mA)/m2 and forIrrλ could be W (or mW)/cm2. Ex-perimental results are shown in Fig. 4. It can be seen thatthe maximum IPCE value occurs at the energy of 2.75 eVapproximately. This value is close to the band gap value ofCdS , which is around 2.4 eV. It means the light is travel-ing thorough CdS layer and is being absorbed by the P3OTlayer. Both layers met the objective for they were chosen asmaterials for PV applications.
A systematic analysis of electrical characterization lets usget mathematical models to describe hybrid HJs electrical
behavior. With this systematic study it was demonstratedthat Irr level plays an important roll over the PV perfor-mance of CdS/P3OT hybrid HJs. Physical and electrical pa-rameters involved in the mathematical models, describe HJelectrical behavior with high confidence level. The obtainedexperimental-theoretical models are a very useful and pow-erful simulation tool, which can be used to a continuous im-provement. The internal photon to electron conversion effi-ciency depends on the wavelength of the incident light. Phys-ical, optical and mechanical characteristics of P3OT and CdSmaterials are highly compatible to prepare devices for PV ap-plication.
The authors thank Cecilia Lopez-Mata for CdS/P3OT solarcell sample preparation. The financial support from DGAPA-UNAM and CONACyT is gratefully acknowledged.
1. Oscar H. Salinas, C. Lopez-Mata, H. Hu, and M.E. Nicho,Sol.Energy Mater. Sol. Cells90 (2006) 2421.
2. D. Gebeyehuet al., Synthetic Metals118(2001) 1.
3. P. Rappaport,RCA Rev.20 (1959) 373.
4. S.M. Sze,Physics of Semiconductor Devices2nd Edition. (JohnWiley and Sons, New York, 1981).
5. H. Spanggaard, and F.C. Krebs,Sol. Energy Mater. Sol. Cells83 (2004) 125.
6. K.M. Coakley and M.D. McGehee,Chem. Mater.16 (2004)4533.
7. J.H. Lee, J.H. Park, J.S. Kim, D.Y. Lee, and K. Cho,OrganicElectronics10 (2009) 416.
8. Huang Zhong Yu and Jun Biao Peng,Organic Electronics9(2008) 1022.
9. Hailin Hu, Sheng-Chin Kung, Li-Mei Yang, M.E. Nicho, andR.M. Penner,Sol. Energy Mater. Sol. Cells93 (2009) 51.
10. G. Li et al., Nature Mater.4 (2005) 864.
11. Oscar H. Salinas, C. Lopez-Mata, H. Hu, M.E. Nicho, and A.Sanchez,Sol. Energy Mater. Sol. Cells90 (2006) 760.
12. P.K. Nairet al., Sol. Energy Mater. Sol. Cells52 (1998) 313.
13. M.T.S. Nair, P.K. Nair, R.A. Zingaro, and E.A. Meyers,J. Appl.Phys.75 (1994) 1557.
14. C. Lopez-Mata, M.E. Nicho, Hailin Hu, G. Cadenas-Pliego,and E. Garcıa-Hernandez,Thin Solid Films490(2005) 189.
15. J.S. Kimet al., J. Appl. Phys.84 (1998) 6859.
Rev. Mex. Fıs. E57 (1) (2011) 73–77